JLMN-Journal of Laser Micro/Nanoengineering Vol. 11, No. 1, 2016
Laser Cutting of Carbon Fiber Reinforced Plastics (CFRP and CFRTP) by IR Fiber Laser Irradiation
Hiroyuki Niino*1,2, Yoshihisa Harada*1,2, Kenji Anzai*1,3, Masafumi Matsushita*1,4, Koichi Furukawa*1,4, Michiteru Nishino*1,5, Akira Fujisaki*1,6, and Taizo Miyato*1,6
*1 Advanced Laser and Process Technology Research Association (ALPROT), Tokyo, Japan, *2 National Institute of Advanced Industrial Science and Technology (AIST), Tsukuba, Japan,
*3 AMADA MIYACHI CO., LTD., Noda, Japan, *4 Shin Nippon Koki Co., Ltd., Osaka, Japan,
*5 Mitsubishi Chemical Corporation, Tokyo, Japan, *6 Furukawa Electric Co., Ltd., Chiba, Japan
We report here laser cutting of carbon fiber reinforced plastic (CFRP) with an IR fiber laser (average power: 2 - 3 kW). The CFRP samples contain thermoplastic resin (CFRTP; carbon fiber reinforced thermo-plastic) or thermosetting resin as binding plastic. Well-defined laser cutting free of debris around the groove was performed for various type of CFRP plates by the laser irradiation with a fast beam galvanometer scanner on a multiple-scan-pass method. The laser-induced damage in the samples was observed and analyzed by microscopic X-ray Computed Tomography. Laser cutting with a high speed beam scanning exhibits a clean top and excellent sidewall quality along with a negligible heat-affected zone.
Keywords: laser micromachining, laser ablation, cw IR fiber laser, CFRTP and CFRP composite
1. Introduction Laser-induced cutting of various materials has led to
inventions of numerous industrial processes that have redefined the speed of production-line manufacturing and the strength of industrial manufacturing applications. Reliable systems composed of rapid and easy operations with excellent repeatability can be designed with solid-state lasers. The laser cutting process achieves high-precision cuts with narrow kerfs where complex contours demand precise, fast and force-free processing [1, 2]. In particular, considerable attention has been given towards the cutting of carbon fiber reinforced plastic (CFRP) and carbon fiber reinforced thermo-plastic (CFRTP), composite materials of resin matrices and reinforced carbon fibers, since, in spite of the difficulty involved, they are high strength, and yet lightweight materials, and is increasingly being used for various applications in automotive and aerospace fields. The use of lasers for these composite materials can involve several approaches, such as fiber laser processing [3 26], UV laser processing [15, 21, 27-38], picosecond laser micromachining [39-48], femtosecond laser micromachining [43, 49, 50], disk laser processing [51, 52], YAG laser processing [53-64], CO2 laser processing [5, 19, 22, 24-26, 57, 65-77], and theoretical model/analysis [78-84]. In addition, another advantage of laser processes is flexibility of groove shaping in accord with laser scanning tracks. To explore the possibility of 3D laser processing, cutting of CFRP for a three-dimensional molded sample was performed with a five-axis laser cutting machine .
In this paper, we report on the laser cutting of CFRTP and CFRP plates with a cw fiber near-IR laser (= 1084 nm). Well-defined cutting free of debris around the groove
was achieved for CFRTP and CFRP by the laser irradiation with a fast beam galvanometer scanner on a multiple-scan-pass method [35, 811, 16, 17, 36, 55, 71]. The laser-induced damage in the samples was observed to estimate heat-affected zone (HAZ), by microscopic X-ray Computed Tomography (X-CT).
Two different types of samples of three-mm-thick CFRTP plates were employed for the laser cutting. These were prepared by injection molding (chopped PAN-type carbon fiber (Cf= 30 wt%) in ABS-resin (ABS; co-polymer of acrylonitrile-butadiene-styrene, Toray Industries Inc.) and PPS resin (polyphenylene sulfide, Toray Industries Inc.).
Three-mm-thick CFRP plates of PAN-based carbon fiber was also used for the laser cutting. The CFRP sample used in this study was commercially available prepreg laminate consisting of thermoset epoxy resin with PAN-based carbon fibers. The lamina consists of unidirectional fiber stacking parallel and perpendicular to the fiber direction (cross-ply 0/90, 12-ply layers, Cf= 70%).
We used a near-IR laser (Furukawa Electric, Yb-doped fiber laser, wavelength = 1084 nm, multi-mode (fiber core diameter: 50 m), average power P= 2 - 3 kW). The laser was operated in the cw-mode or the qcw-mode (duty 40 %, repetition rate 800 Hz). The laser beam on the sample surface was scanned with a galvanometer scanner by multiple-scan-pass irradiation in the air (scanning speed: 3.6 m s-1, without assist gas). The beam was focused on the laser-incident sample surface with an f-theta lens (f= 306 mm). In addition, the cutting procedure of double scanning
JLMN-Journal of Laser Micro/Nanoengineering Vol. 11, No. 1, 2016
line with the gap of 0.1 mm was also employed for the complete cutting of three-mm-thick CFRP-epoxy sample in order to acquire wide kerf width of the groove.
The internal damages of laser-cut samples were observed with a micro X-ray Computed Tomography system (Yamato Science Co.; TDM1000H-S/TDM1600H-II, X-ray filament: LaB6).
3. Results and Discussion 3.1 Laser cutting property of CFRTP (thermo-plastic resin)
The cross-sectional and 3D images of CFRTP-ABS sample after cw fiber laser irradiation on a multiple-scan-pass method are shown in Fig. 1. Laser scanning speed was set at 3.6 m s-1. As the laser-pass-number at cw 2kW-laser irradiation increases, the depth of cutting grooves increases proportionally (Fig. 1(a)). In addition, the observation from the direction perpendicular to the grooves proves that the depth of a groove is uniform until the plate was completely cut. The kerf width of the groove on the laser beam incident surface is estimated to be 500 m. The internal kerf of the groove in bulk region is ca. 200 m, as shown in Fig. 1(a). The 3D image of CFRTP-ABS shows only a few debris deposited on the laser-incident sample surface (Fig. 1(b)) [23, 33].
(b) Fig. 1 X-CT image of three-mm-thick CFRTP-ABS plate cut by cw fiber laser irradiation on a multiple-scan-pass method. Laser scanning speed on the sample was set at 3.6 m s-1; Laser-pass-number: 1, 2, 5, 10, 15. (a) cross-sectional image of the CFRTP-ABS plate, (b) volume rendering 3D-image.
Figure 2 shows the cutting depth of three-mm-thick CFRTP-PPS and CFRTP-ABS plates plotted as the function of the laser pass-number. Linear relation between the cutting depth and laser pass-number was observed for both of CFRTP-PPS and CFRTP-ABS. The complete cutting of the CFRTP-PPS and CFRTP-ABS plates required the multiple-scan-pass irradiation of 27 passes and 15 passes, respectively, at the scanning speed of 3.6 m s-1 at cw 2kW-laser irradiation.
We have already reported that other types of CFRTP in the resin of, such as, polycarbonate (CFRTP-PC) and polyamide (CFRTP-PA, nylon6) also indicate the linear relation with the fiber laser irradiation [3, 8-10]. The above results indicate that constant etching rate as far as the thickness of 3 mm was acquired for various CFRTP samples; the depth of a groove of CFRTP samples can be precisely controlled by the laser pass-number.
0 5 10 15 20 25 30Laser-pass-number
Fig. 2 Cutting depth of the three-mm-thick CFRTP plates by cw fiber laser irradiation on a multiple-scan-pass method (cw 2kW-laser irradiation). Laser scanning speed was set at 3.6 m s-1; red-colored circle: CFRTP-ABS (ABS resin), blue-colored circle: CFRTP-PPS (polyphenylene sulfide).
High resolution X-CT images of the CFRTP-ABS and CFRTP-PPS samples are shown in Figs. 3 and 4. The internal kerf of the groove in the bulk region is ca. 200 m, as shown in Fig. 3(a), so that the aspect ratio of the groove is ca. 15. Figure 4(a) indicates that the internal kerf of CFRTP-PPS is ca. 100-200 m.
Cross-sectional image of Fig. 3(a) clearly shows the formation of micron-sized voids (dark spots in the image) in the subsurface of internal wall at the groove. As the micron-sized voids are produced by thermal damage during the laser irradiation, the voids are present on the entire surface of the internal wall (Fig. 3(b)). It is worth noted that the micron-sized voids appear only within the 100-m-thick surface layer of the internal wall of the groove, suggesting that thermal damage as HAZ (heat-affected zone) during the laser irradiation of the CFRTP-ABS sample was effectively suppressed. The formation of micron-sized voids of CFRTP-PPS sample was observed within the 130-m-thick surface layer of the internal wall of the groove (Fig. 4(a)). Laser irradiation on CFRTP-PC and CFRTP-PA also induces micron-sized void formation within the 100-m-thick surface layer of the internal wall of the groove [3, 8-10].